Dislocation theory

**Dislocation** **theory**

Subjects of interest

• Introduction/Objectives

• Observation of dislocation

• Burgers vector and the dislocation loop

• **Dislocation** in the FCC, HCP and BCC lattice

• Stress fields and energies of dislocations

• Forces on dislocations and between dislocations

Chapter 5

Suranaree University of Technology May-Aug 2007

Tapany Udomphol

**Dislocation** **theory**

Subjects of interest (continued)

• **Dislocation** climb

• Intersection of dislocations

• Jogs

• **Dislocation** sources

• Multiplication of dislocations

• **Dislocation**-point defect interactions

• **Dislocation** pile-ups

Chapter 5

Suranaree University of Technology May-Aug 2007

Tapany Udomphol

Objectives

• This chapter emphasises the understanding of the

effects of dislocation behaviour on FCC, BCC and HCP

crystal structures.

• This includes the interaction of dislocations such as

climb, jogs, intersection and multiplication of dislocations

and the roles of dislocations on plastic deformation of

metals.

Suranaree University of Technology May-Aug 2007

Tapany Udomphol

Introduction

**Dislocation**s introduce imperfection into the structure and therefore

these could explain how real materials exhibit lower yield stress value

than those observed in **theory**.

**Dislocation**s

51450 x

Produce

imperfection in

crystal structures

• Lower the yield stress from

theoretical values.

• Produce plastic deformation

(strain hardening).

• Effects mechanical properties

of materials.

Suranaree University of Technology May-Aug 2007

Tapany Udomphol

Observation of dislocations

A variety of techniques have been used to observe dislocations in

the past 20 years to aid the better understanding of dislocation

behaviour.

Chemical (etch–pit) technique

• Using etchant which forms a pit at the

point where a dislocation intersect the

surface.

• Preferential sites for chemical attack are

due to strain field around dislocation sites

(anodic).

• Can be used in bulk samples but limited in

low dislocation density crystal (10 4 mm -2 ).

Note: Pits are 500 A o apart and with

the dislocation density of 10 8 mm -2 .

5000 x

Etch pits on slip bands in alpha

brass crystals

Suranaree University of Technology May-Aug 2007

Tapany Udomphol

Decoration of dislocation technique

A small amount of impurity is added to form precipitates after

suitable heat treatment to give internal structure of the

dislocation lines.

• Hedges and Mitchell first used

photolytic to decorate dislocation in

AgBr.

• Rarely used in metals but in ironic

crystals such as AgCl, NaCl, KCl

and CaF 2 .

Hexagonal network of dislocations

in NaCl detected by a decoration

technique.

Suranaree University of Technology May-Aug 2007

Tapany Udomphol

Transmission electron microscope (TEM)

TEM is the most powerful technique used to study dislocations.

• A thin foil of 100 nm is prepared using

electropolishing from a ~1 mm thick sheet.

• This thin foil is transparent to electrons in

the electron microscope and this makes it

possible to observed dislocation

networks, stacking faults, dislocation

pile-ups at grain boundaries.

• By using the kinematic and dynamic

theories of electron diffraction it is possible

to determine the dislocation number,

Burgers vectors and slip planes.

32500 x

**Dislocation** network in cold-worked

aluminium.

Note: The sampling area is small therefore the properties

observed cannot represent the whole materials.

Suranaree University of Technology May-Aug 2007

Tapany Udomphol

X-ray ray microscopy

• Using an X-ray technique to detect dislocation structure.

• The most common techniques are the Berg-Barret reflection

method and the Lang topography method.

• The resolution is limited to 10 3 dislocations/mm 2 .

Suranaree University of Technology May-Aug 2007

Tapany Udomphol

Burgers vector and the

dislocation loop

Burgers vector is the most

characteristic feature of a

dislocation, which defines the

magnitude and the direction of slip.

• Edge Burgers vector is to the

dislocation line.

• Screw Burgers vector is // to the

dislocation line.

• Both shear stress and final

deformation are identical for both

situations.

Macroscopic deformation produced by glide of

(a) edge dislocation and (b) screw dislocation.

Note: Most dislocations found in crystalline materials are

probably neither pure edge or pure screw but mixed.

Suranaree University of Technology May-Aug 2007

Tapany Udomphol

**Dislocation** loops

**Dislocation**s in single crystals are straight lines. But in general,

dislocations appear in curves or loops, which in three

dimensions form and interlocking dislocation network.

• Any small segments of the dislocation

can be resolved into edge and screw

components.

• Ex: pure screw at point A and pure edge

at point B where along most of its length

contains mixed edge and screw. But with

the same Burgers vector.

**Dislocation** loop lying in

a slip plane.

Suranaree University of Technology May-Aug 2007

Tapany Udomphol

Burgers circuit

Burgers circuit is used to define the Burgers vector of dislocation.

(a)

Burgers circuits

around edge

dislocation

(b)

Burgers circuits

around screw

dislocation

• If we trace a clockwise path from start to finish, the closure

failure from finish to start is the Burgers vector b of the

dislocation, see fig (a).

• A right-handed screw dislocation, fig (b), is obtained

when transversing the circuit around the dislocation line and

we then have the helix one atomic plane into the crystal.

Suranaree University of Technology May-Aug 2007

Tapany Udomphol

Cross slip

In FCC cubic metals, the screw dislocations move in {111} type

planes, but can switch from one {111} type plane to another if it

contains the direction of b. This process is called cross-slip.

**Dislocation**

S

Cross slip in a face-centred cubic crystal.

Cross slip on the polished surface

of a single crystal of 3.25% Si iron.

• A screw dislocation at S is free to

glide in either (111) or (111)

closed-packed planes.

• Double cross slip is shown in (d).

Suranaree University of Technology May-Aug 2007

Tapany Udomphol

**Dislocation** dissociation

**Dislocation** dissociation occurs when the strength of

dislocation is more than unity. The system becomes unstable

dislocation therefore dissociate into two dislocation.

Note: **Dislocation** of unit strength is a dislocation with a Burgers

vector equal to one lattice spacing.

The dissociation reaction b 1 b 2 + b 3 will occur

when b 1 2 > b2 2 + b3 2 .

• A dislocation of unit strength has a minimum energy

when its Burgers vector is parallel to a direction of closest

atomic packing.

• In close-packed lattices, dislocations with strength less

than unity are possible. therefore crystals always slip in

the close-packed direction.

Suranaree University of Technology May-Aug 2007

Tapany Udomphol

**Dislocation**s in FCC lattice

• Slip occurs in the FCC lattice on the {111} plane in the direction

and with a Burgers vector (a/2)[110].

• The {111} planes are stacked on a close packed sequence ABCABC

and vector b = (ao /2)[101] defines one of the observed slip direction,

which can favourably energetically decompose into two partial

dislocations.

b

1

a

o

2

→ b

2

[ 101]

+ b

→

3

a

o

6

a

o [ 211]

+ [ 112]

Shockley partials

This Shockley partials creates a

stacking fault ABCAC/ABC.

6

Extended dislocation

Fully slipped

Faulted

region

No slip

Dissociation of a dislocation to

two partial dislocations.

Suranaree University of Technology May-Aug 2007

Tapany Udomphol

Dissociation of a dislocation into two

partial dislocations

• The combination of the two partials AC and

AD is known as an extended dislocation.

• The region between them is a stacking

fault which has undergone slip.

• The equilibrium of these partial dislocations

depends on the stacking fault energy.

Group of stacking fault in 302 stainless

steel stopped at boundary

Extended dislocation

Fully slipped

Faulted

region

No slip

www.msm.cam.ac.uk

Stacking fault

Suranaree University of Technology May-Aug 2007

Tapany Udomphol

Stacking faults

The wider region between partial dislocation,

the lower stacking fault energy

• Characteristics of metals with

low SPF;

1) Easy to strain harden

2) Easy for twin annealing to occur

3) Temperature dependent flow

stress

• Aluminium – high stacking fault energy

more likely to cross slip.

• Copper – lower stacking fault energy

cross slip is not prevalent.

Partial

dislocations

Stacking fault

Typical values of stacking fault energy

Metal Stacking fault energy (mJ m -2 )

Brass

303 stainless steel

304 stainless steel

310 stainless steel

Silver

Gold

Copper

Nickel

Aluminium

Slip plane

Model of a stacking fault.

Suranaree University of Technology May-Aug 2007

Tapany Udomphol

Frank partial dislocations

Frank partial dislocations are

another type of partial dislocation in

FCC lattice, which provide

obstacles to the movement of other

dislocations.

Frank partial dislocation or sessile

dislocation.

• A set of (111) plane (viewed from the edge) has a missing middle A

plane with a Burgers vector (a o /3) [111] perpendicular to the central

stacking fault.

• Unlike perfect dislocation, Frank partial dislocation cannot move

by glide (sessile dislocation) but by diffusion of atom.

Suranaree University of Technology May-Aug 2007

Tapany Udomphol

Lomer-Cortrell barrier

Intersection of {111} plane during

duplex slip by glide of dislocations is

called Lomer-Cortrell barrier.

Ex: consider two perfect dislocations

lying in different {111} planes and

both parallel to the line of intersection

of the {111} plane.

a

o

2

[ 101]

+

a

o

2

[ 110]

[ 011]

Lomer-Cortrell barrier

The new dislocation obtained has reduced energy.

→

Suranaree University of Technology May-Aug 2007

a

o

2

Tapany Udomphol

**Dislocation**s in HCP lattice

• Slip occurs in the HCP lattice on the basal (0001) plane in the

direction.

• The basal (0001) plane the close packed of a sequence ABABAB

and a Burgers vector b = (a o /3)[1120].

• **Dislocation**s in the basal plane can reduce their energy by

dissociating into Shockley partials according to the reaction.

a

o

3

[ 1120]

→

a

o

3

[ 1010]

[ 0110]

The stacking fault produced by this reaction lies in the basal

plane, and the extended dislocation which forms it is confined to

glide in this plane.

Suranaree University of Technology May-Aug 2007

+

a

o

3

Tapany Udomphol

**Dislocation**s in BCC cubic lattice

• Slip occurs in the BCC lattice on {110}, {112}, {123} planes in the

direction and a Burgers vector b = (a o /2)[111].

Cottrell has suggested a dislocation reaction which appears to cause

immobile dislocations. (ao /2[001] in iron) leading to a crack

nucleus formation mechanism for brittle fracture.

a

o

2

[ 111]

+

a

o

2

[ 111]

→

the dislocation is immobile since

the (001) is not a close-packed slip

plane, the (001) plane is therefore

the cleavage plane when brittle

fracture occurs.

a

o

[ 001]

b = a[

001]

a

[ 111]

2

a

[ 111]

2

(101) Slip plane

(101) Slip plane

Applied stress

(001) Cleavage plane

Slip on intersecting (110) plane.

Suranaree University of Technology May-Aug 2007

Tapany Udomphol

a

2

σ

σ

a

111

2

[ 111]

+ [ ] → a[

001]

Cleavage knife crack of length c

for displacement nb

Stress fields of dislocations

A dislocation is surrounded by an elastic stress field that

produces forces on other dislocations and results in interaction

between dislocations and solute atoms.

• The cross section of an elastic cylindrical

piece (dashed line) has been distorted after

an edge dislocation running through point O

parallel to the z axis (blue line).

• The strain is zero in the z axis and

therefore can be treated in plane strain (x-y).

• The stresses vary inversely with distance

from the dislocation line and become

infinite at r = 0.

−τ

ob

sinθ

…Eq. 1 σ r = σ θ =

r

• The shear stress ττττ xy is a maximum

in the slip plane, when y = 0.

2 2 ( x − y )

2 2

( x + y

Suranaree University of Technology May-Aug 2007

τ

Tapany Udomphol

xy

= τ

o

bx

y

r

P

O

Q

θθθθ

A’ A

r o

Deformation of a circle containing

an edge dislocation.

)

2

b

x

…Eq. 2

Strain energies of dislocations

The strain energy involved in the

formation of an edge dislocation can

be estimated from the work involved in

displacement the cut OA a distance b

along the slip plane.

U

=

2

Gb

ln

4π ( 1−ν

)

The strain energy of a screw

dislocation is given by

U

2

Gb

4π

r

r

o

r

r

1

o

…Eq. 3

1

= ln

…Eq. 4

Note: the total strain energy is the

sum of elastic strain energy and

the core energy of dislocation.

Suranaree University of Technology May-Aug 2007

y

r

P

O

Q

θθθθ

A’ A

r o

Deformation of a circle containing

an edge dislocation.

The dislocation energy per unit

length simplifies to

Tapany Udomphol

2

Gb

U = …Eq. 5

2

b

x

Forces on dislocation

ds

b

dl

Force acting on a dislocation line.

• A dislocation line moving in the

direction of its Burgers vector under the

influence of a uniform shear stress ττττ.

• The force per unit length of dislocation F ;

dW

F = = τb

dlds

…Eq. 6

• This force is normal to the dislocation

line at every point along its length and is

directed toward the unslipped part of

the glide plane.

• The Burgers vector is constant along

the curved dislocation line.

Suranaree University of Technology May-Aug 2007

Tapany Udomphol

Forces between dislocations

• **Dislocation**s of opposite sign on the same slip plane will

attract each other, run together, and annihilate each other.

• **Dislocation**s of alike sign on the same slip plane will repel

each other

The radial force F r between

two parallel screw dislocations

Fr = τ θz

b

2

Gb

=

2πr

…Eq. 7

Parallel screw (same sign) +

Aniparallel screw (opposite sign) -

The radial and tangential

forces between two parallel

edge dislocations

F r

2

Gb 1

2π

( 1−ν

) r

2

Gb sin 2θ

2π

( 1−ν

) r

Suranaree University of Technology May-Aug 2007

=

Tapany Udomphol

, F

θ

=

…Eq. 8

**Dislocation** climb

**Dislocation** climb is a non conservative movement of dislocation

where and edge dislocation can move out of the slip plane onto a

parallel directly above or below the slip plane.

• Climb is diffusion-controlled (thermal activated) and occurs more

readily at elevated temperature. important mechanism in creep.

• Positive direction of climb is when

the edge dislocation moves upwards.

Removing extra atom (or adding vacancy

around ). Compressive force

produces + climb.

• Negative direction of climb is when

the edge dislocation moves downwards.

Atom is added to the extra plane. Tensile

forces to produce – climb.

(a) Diffusion of

vacancy to edge

dislocation.

(b) **Dislocation**

climbs up one

lattice spacing.

Note: Glide or slip of a dislocation is the direction parallel to its

direction whereas climb of dislocation is in the vertical direction.

Suranaree University of Technology May-Aug 2007

Tapany Udomphol

Intersection of dislocations

The intersection of two dislocations produces a sharp

break (a few atom spacing in length) in dislocation line.

This break can be of two types;

• Jog is a sharp break in the dislocation

moving it out of the slip plane.

• Kink is a sharp break in the dislocation line

which remains in the slip plane.

Note: **Dislocation** intersection mechanisms play an important

role in the strain hardening process.

Suranaree University of Technology May-Aug 2007

Tapany Udomphol

Jogs and Kinks

Jogs are steps on the dislocation which move it from one atomic

slip plane to another.

Kinks are steps which displace it on the same slip plane.

(a), (b) Kinks in edge and

screw dislocations

(c), (d) Jogs in edge and

screw dislocations.

Suranaree University of Technology May-Aug 2007

Tapany Udomphol

Intersection of two dislocations

1) Intersection of two dislocations with

Burgers vectors at right angle to each other.

• An edge dislocation XY with Burgers vector b 1

is moving on plane P xy and cuts through

dislocation AB with Burgers vector b 2 .

• The intersection causes jog PP’ in dislocation

AB parallel to b 1 and has Burgers vector b 2 .

and with the length of the jog = b 1 .

• It can readily glide with the rest of dislocation.

Note: b 1 is normal to AB and jogs AB, while

b 2 is parallel to XY and no jog is formed.

Intersection of two

edge dislocations

Suranaree University of Technology May-Aug 2007

Tapany Udomphol

b 2

b 1

Intersection of two dislocations

2) Intersection of two dislocations with

Burgers vectors parallel to each other

• Both dislocations are jogged.

• The length of jog PP’ is b 1 and

the length of jog QQ’ is b 2 .

• The jogs both have a screw

orientation and lie in the original

slip plane. This is called Kink.

not stable.

Before

intersection

After

intersection

Intersection of edge dislocations

with parallel Burgers vectors.

Suranaree University of Technology May-Aug 2007

Tapany Udomphol

Intersection of two dislocations

3) Intersection of edge and

screw dislocations.

Intersection produces a jog with an

edge orientation on the edge

dislocation and a kink with an edge

orientation on the screw dislocation.

4) Intersection of two screw

dislocations.

The intersection produces jogs

of edge orientation in both screw

dislocations. very important in

plastic deformation.

Note: at temperature where climb

cannot occur the movement of screw

dislocation is impeded by jogs.

Suranaree University of Technology May-Aug 2007

Tapany Udomphol

Jogs

• A stable jog length of the dislocation line energy of the crystal

(a) Many intersections occur when a

screw dislocation encounter a forest of

screw dislocations. producing

vacancy jogs and/or interstitial jogs.

(b) Jogs act as pinning points and

cause dislocations to bow out with

the radius R when the shear stress

ττττ is applied.

(c) At some critical radius R c the ττττ

required to further decrease R > the

stress needed for non-conservative

climb. Then the dislocation will move

forward leaving a trail of vacancies

(interstitials) behind each jog.

(a) Straight dislocation under zero stress.

(b) **Dislocation** bowed out in slip plane

between the jogs due to applied shear stress.

(c) Movement of dislocation leaving trails of

vacancies behind the jogs.

Movement of jogged screw dislocation

Suranaree University of Technology Tapany Udomphol

May-Aug 2007

Superjogs

Superjog is a jog that has more than one atomic slip plane spacing high.

As the stress increases, the dislocation bows out between the

superjogs, generating dislocation dipoles and later break into

isolated loops.

(a) **Dislocation** dipole.

(b) Elongated loop and

jogged dislocation.

(c) Row of small loops.

Formation of dislocation loops from a dislocation dipole

Suranaree University of Technology May-Aug 2007

Tapany Udomphol

**Dislocation** Sources

• All metals initially contain an appreciable number of

dislocations produced from the growth of the crystal from

the melt or vapour phase.

• Gradient of temperature and composition may affect

dislocation arrangement.

• Irregular grain boundaries are believed to be responsible

for emitting dislocations.

• **Dislocation** can be formed by aggregation and collapse of

vacancies to form disk or prismatic loop.

• Heterogeneous nucleation of dislocations is possible from

high local stresses at second-phase particles or as a result

of phase transformation.

Suranaree University of Technology May-Aug 2007

Tapany Udomphol

Multiplication of dislocations

Frank & Read proposed that dislocations

could be generated from existing dislocations.

• The dislocation line AB bulges out

(A and B are anchored by impurities)

and produces slip as the shear

stress ττττ is applied.

• The maximum ττττ for

semicircle dislocation

bulge, fig (b)

Gb

τ ≈ ≈

2R

Gb

l

• Beyond this point, the dislocation loop

continues to expand till parts m and n

meet and annihilate each other to form a

large loop and a new dislocation.

Note: Repeating of this process producing a

dislocation loop, which produces slip of one

Burgers vector along the slip plane.

The operation of Frank-Read source

Frank Read source in a silicon crystal

Suranaree University of Technology May-Aug 2007

**Dislocation**-point **Dislocation** point defect interactions

Point defect and dislocation will interact elastically and

exert forces on each other.

If the solute atom is

larger than the

solvent atom (εεεε > 1)

If the solute atom is

smaller than the

solvent atom (εεεε < 1)

Negative interaction energy attraction

Positive interaction energy repulsion

The atom will be repelled from the

compressive side of a positive edge

dislocation and will be attracted to the

tension side.

The atom will be attracted to the

compression side.

• Vacancies will be attracted to regions of compression.

• Interstitials will be collected at regions of tension.

Suranaree University of Technology May-Aug 2007

Tapany Udomphol

**Dislocation** pile-ups pile ups

**Dislocation**s often pile up

on slip planes at barriers

i.e., grain boundaries or

second phase particles.

High stress concentration on the

leading dislocations in the pile-up.

If the pile-up stress > theoretical shear stress yielding

A pile-up of n dislocations along

a distance L can be considered

as a giant dislocation with a

Burgers vector nb.

**Dislocation** pile-ups at an obstacle.

The breakdown of a barrier occur by

1) Slip on a new plane.

2) Climb of dislocation around the

barrier.

3) Generation of high enough tensile

stress to produce a crack.

Suranaree University of Technology May-Aug 2007

Tapany Udomphol

References

• Dieter, G.E., Mechanical metallurgy, 1988, SI metric edition,

McGraw-Hill, ISBN 0-07-100406-8.

• Sanford, R.J., Principles of fracture mechanics, 2003, Prentice

Hall, ISBN 0-13-192992-1.

• W.D. Callister, Fundamental of materials science and

engineering/ an interactive e. text., 2001, John Willey & Sons, Inc.,

New York, ISBN 0-471-39551-x.

• Hull, D., Bacon, D.J., Introduction to dislocations, 2001, Forth

edition, Butterworth-Heinemann, ISBN 0-7506-4681-0.

Suranaree University of Technology May-Aug 2007

Tapany Udomphol